Measurements of stress-optic coefficient and Young's modulus in
PMMA fibers drawn under different conditionsMeasurements of
stress-optic coefficient and Young's modulus in PMMA fibers drawn
under different conditions
Marcin K. Szczurowski1, Tadeusz Martynkien1, Gabriela
Statkiewicz-Barabach1, Lutful Khan2,
David J. Webb2, Chenchun Ye3, Janice Dulieu-Barton3, Waclaw
Urbanczyk1,*
1Institute of Physics, Wroclaw Univ. of Technology, Wyb.
Wyspianskiego 27, 50-370 Wroclaw, Poland,
*
[email protected]
2Photonics Research Group, Aston University, Birmingham, B4 7ET, UK
3Univ. of Southampton, School of Engineering Sciences, Highfield,
Southampton, SO17 1BJ, UK
ABSTRACT
We have systematically measured the differential stress-optic
coefficient, ΔC, and Young’s modulus, E, in a number of PMMA fibers
drawn with different stress, ranging from 2 up to 27 MPa. Effect of
temperature annealing on those parameters was also investigated. ΔC
was determined in transverse illumination by measuring the
dependence of birefringence on additional axial stress applied to
the fiber. Our results show that ΔC in PMMA fibers has a negative
sign and ranges from -4.5 to -1.5×10-12 Pa-1 depending on the
drawing stress. Increase of the drawing stress results in greater
initial fiber birefringence and lower ΔC. The dependence of ΔC and
initial birefringence upon drawing stress is nonlinear and
gradually saturates for higher drawing stress. Moreover, we find
that ΔC is linearly proportional to initial fiber birefringence and
that annealing the fiber has no impact on the slope of this
dependence. On the other hand, no clear dependence was observed
between the fiber drawing stress and the Young's modulus of the
fibers as measured using microscopic digital image correlation with
the fibers tensioned using an Instron tension tester.
Keywords: polymer fibers, birefringence, stress-optic coefficient,
Young’s modulus
1. INTRODUCTION PMMA is a very popular polymer widely used in
photonic technology for fabrication of micro-optical elements,
integrated devices and optical fibers. There are many literature
inconsistencies concerning its mechanical constants, especially the
differential stress-optic coefficient ΔC=C1-C2. Measurements
performed in PMMA discs (18mm diameter, 10mm thick) showed ΔC equal
to -3.3×10-12 Pa-1 [1], but in [2] the measurements carried out in
discs of different size (13.03 mm diameter, 2.85mm thick) gave a
value of ΔC=5.5×10-10 Pa-1. Another quite different result was
reported in [3], ΔC=1.08×10-10 Pa-1. Very systematic studies of the
optical and mechanical properties of bulk PMMA (Plexiglas 55) are
presented in [4]. In particular, the strain-optic coefficients for
this material have been measured p11=0.300, p12=0.297 in [4], which
leads to a calculated value of ΔC = -2.30×10-12 Pa-1, assuming the
following material constants: refractive index n=1.4904 at a
wavelength λ= 690 nm, Young’s modulus E=3 GPa, and Poisson’s ratio
ν=0.37. The purpose of this study is to measure systematically the
differential stress-optic coefficient and Young's modulus in a set
of PMMA fibers drawn under different conditions. The fibers used in
this study were all drawn from homogeneous, nominally pure PMMA
rods obtained from AMARI plastics. The mean molecular weight was
determined by gas permeation chromatography to be 87,000. To
prevent the preforms from bubbling in the draw tower oven, they
were annealed at 80°C for 48 hours immediately prior to fiber
drawing. The fibers were all drawn with a hot-zone temperature of
181±2°C and the fiber tension controlled by adjusting the preform
feed and fiber take-up rates. A selection of the investigated fiber
samples was annealed at 100°C for 20 hours and the effect of
annealing on differential stress optic coefficient and Young’s
modulus was also studied in this work.
2. MESUREMENT OF STRESS-OPTIC COEFFICIENT To determine ΔC=C1-C2, we
measured the dependence of fiber birefringence upon additional
axial stress applied to the fiber, σz
applied. The drawing stress and geometrical parameters of the
examined fibers are gathered in Table 1. To measure the fiber
birefringence in the direction perpendicular to the symmetry axis,
we used a system employing a Senarmont compensation principle. The
system was composed of microscope objective, CCD camera, polarizer,
motorized analyzer,
Photonic Crystal Fibers IV, edited by Kyriacos Kalli, Waclaw
Urbanczyk, Proc. of SPIE Vol. 7714, 77140G · © 2010 SPIE · CCC
code: 0277-786X/10/$18 · doi: 10.1117/12.855089
Proc. of SPIE Vol. 7714 77140G-1
achromatic quarterwave plate, and a bright LED source with central
wavelength at 526 nm, as it is shown in Fig.1. The investigated
fibers were immersed in index matching liquid to avoid light
refraction at the edges. Intrinsic fiber birefringence arising
during the drawing process or introduced by applied axial stress,
causes retardation between wavefronts of orthogonal polarizations
Σx(x) and Σy(x), when the fiber is illuminated perpendicularly to
its symmetry axis. To determine the retardation distribution across
the fiber R(x)=Σx(x)-Σy(x), a computer controlled CCD camera took a
series of pictures for different positions of a rotatable analyzer.
After appropriate processing of a series of collected photographs,
the retardation maps were obtained for all investigated
fibers.
Table 1. Parameters of the investigated fibers. All annealed fibers
are indicated by an apostrophe. Annealing temperature was 100°C and
duration 20 h.
Fiber sample
Measured diameter
LED
Fig.1. Experimental set-up for measuring retardation distribution
in the PMMA fibers.
∫ −
Proc. of SPIE Vol. 7714 77140G-2
where r0 is the fiber radius, σz(r) is the axial stress, and dR/dx
is a derivative of measured retardation. The differential stress
optic coefficient ΔC can be easily retrieved by applying increasing
axial load to the fiber and finally by plotting the dependence
ΔCσz
calculated versus σz applied with ΔC being a proportionality
coefficient.
An axial stress applied to the fiber induces optical anisotropy
characterized by three principal indices nz, nr, nθ. As it is shown
in earlier publication [5], when axial stress is applied to a fiber
made of uniform material, other stress components in the fiber
cross section are significantly lower than σz (σz >>σr
σz>>σΘ ), which results in the following relation:
).()()( rnrnCr zz Θ−=Δσ (2)
As the investigated fibers are made of uniform PMMA, the inverse
Abel transformation of the measured retardation distribution R(x)
provides directly information about the birefringence induced by
applied axial stress.
To test our measurement and processing method, we first measured ΔC
in a reference silica fiber. Silica is a very well characterized
material thus allowing us to compare the results obtained using our
method with a reliable literature value [6], ΔC= (3.57±0.03) ×10-12
Pa-1 at 526 nm. In Fig.2 phase retardation maps are shown for
unloaded and loaded fiber. In Fig.3b we show the birefringence
distribution reconstructed from the retardation maps measured for
different axial stress applied (Fig.3a). (a) (b)
Fig.2. Phase retardation map measured in silica fiber in transverse
direction: no stress applied (a), 133 MPa stress applied (b).
-60 -40 -20 0 20 40 60 80
0
10
20
30
40
]
x [μm] -80 -60 -40 -20 0 20 40 60 80
-0.5
-0.4
-0.3
-0.2
-0.1
0.0
0.1
0.2
x [μm]
(a) (b)
Fig.3. Phase retardation measured in silica fiber for different
axial stress applied (a) and birefringence reconstructed using the
inverse
Abel transform (b).
By the linear fitting of reconstructed birefringence in pure silica
cladding versus applied stress, we obtained a value for the
stress-optic coefficient of ΔC=(3.52±0.01)×10-12 Pa-1, see Fig.6a.
The measured value is almost the same as the one reported in
literature, which gives confidence in our measurement and
processing methods.
Similar measurements were performed for the PMMA fibers drawn with
different stress (Table 1). In Fig.5b we,
Proc. of SPIE Vol. 7714 77140G-3
show the birefringence distribution reconstructed from the
retardation measured for different axial stress applied (Fig.5a),
σz
applied in the PMMA fiber indicated as 1b, which was drawn using a
relatively small drawing stress of 5.85 MPa.
(a) (b)
Fig.4. Phase retardation map measured in 1b PMMA fiber in
transverse direction for applied axial stress of 2.62 MPa (a)
and
30.9 MPa (b).
-120
-100
-80
-60
-40
-20
0
-0.5
-0.4
-0.3
-0.2
-0.1
0.0
x [mm]
(a) (b)
Fig.5. Phase retardation measured in 1b PMMA fiber for different
axial stress applied (a) and birefringence reconstructed using the
inverse Abel transform (b).
For all investigated PMMA fibers, the applied axial stress was
gradually increased until the fiber broke. As it can be clearly
seen in Fig.5b, the reconstructed distribution of stress–induced
birefringence ΔCσz is not perfectly uniform in the fibers’
cross-sections. An increase of ΔCσz(r) near the fiber edges by
about 10% is most probably caused by the higher cooling rate of the
external layers of the fiber during the drawing process. To
determine ΔC in the polymer fibers, we averaged the measured
distribution of ΔCσz(r) (r) in the fiber cross-section and plotted
the dependence of the averaged σz(r)ΔC = nz - nΘ as a function of
applied stress, see Fig.6a. In order not to obscure this figure, we
show only the results obtained for a few fibers having
significantly different ΔC.
Proc. of SPIE Vol. 7714 77140G-4
0 30 60 90 120 150
-1.25
-1.00
-0.75
-0.50
-0.25
0.00
0.25
0.50
×10-3
Reference silica fiber
-4.5
-4.0
-3.5
-3.0
-2.5
-2.0
-1.5
×10-12
ΔC [P
(a) (b)
Fig.6. Birefringence versus applied stress for silica and PMMA
fibers (a) and ΔC versus drawing stress for PMMA fibers (b).
The birefringence induced by applied axial stress increases
linearly for small values of zσ applied. The stress optic
coefficient ΔC was determined for each PMMA fiber by linear
approximation of the dependence of ΔCσz
calculated (averaged over the fiber cross-section) versus σz
applied for small values of σz applied, with ΔC being a regression
coefficient.
Finally, the dependence of the stress-optic coefficient ΔC upon
drawing stress is presented in Fig.6b. The value of ΔC increases
against σdrawing from -4.5 to -1.5×10-12 Pa-1 in a nonlinear manner
and appears to gradually saturate for high drawing stress. The same
measurements were repeated for the fibers annealed at a temperature
of 100°C for 20 hours. It is interesting that fiber annealing does
not change the general trend in the dependence of ΔC versus
σdrawing, however the saturation effect for annealed fibers occurs
at a greater absolute value of ΔC. Next, we show in Fig.7 the
dependence of ΔC upon residual fiber birefringence, which is
clearly linear with no significant impact of the annealing
process.
-0.0010 -0.0008 -0.0006 -0.0004 -0.0002 0.0000
-5.0
-4.5
-4.0
-3.5
-3.0
-2.5
-2.0
-1.5
ΔC [P
Annealed fibers Not annealed fibers
Fig.7. Dependence of the stress optic coefficient on initial fiber
birefringence
This experimental result shows that the absolute value of the
stress optic coefficient ΔC decreases in the PMMA fibers having
greater initial birefringence, which directly corresponds to a
greater initial ordering of molecules. As the trend line shown in
Fig.9 takes a value of -4.8×10-12 Pa-1 at zero birefringence, we
can estimate ΔC for the bulk PMMA used to draw the fibers,
ΔC=-4.8×10-12 Pa-1.
Proc. of SPIE Vol. 7714 77140G-5
3. MESUREMENT OF YOUNG’S MODULUS
The experimental arrangement shown in Fig.8 was employed to measure
Young modulus in the investigated PMMA fibers. This system is based
on a digital image correlation (DIC) technique using one camera and
allows measurement of the strain-stress curves. The magnified image
of one sample of the POF obtained by the DIC camera using a
microscope with a 3.5x objective is shown in Fig.9a.
POF Pneumatic fibre grip
Microscope
Camera
Fig.8. Experimental set-up for measuring Young’s modulus in PMMA
fibers.
(c) (b) (a)
Fig.9. Image of POF sample indicated as 1a (a), strain map obtained
for stress applied σz applied = 3 MPa (b), strain map obtained
for
σz applied = 28 MPa (c).
Proc. of SPIE Vol. 7714 77140G-6
The length of fiber within the image frame was approximately 3 mm.
Note that images shown in Fig.9b and c have different scales. To
facilitate the DIC measurement, the POFs were covered with white
spray paint and some black powder. Strain maps of the POF sample
with different stresses, as obtained from DIC, are shown in
Fig.9b-c. Representative stress-strain curves for samples 1e and
1e’ are shown in Fig.10. The key influence on the accuracy of the
calculated stress and Young’s modulus is the uncertainty of the
diameter of the POF. The diameters of the POFs were non-uniform
along the sample length due to lack of diameter control in the
drawing process. In addition, the cross sections of some fibres
were not quite circular. A digital micrometer was used to measure
the diameter of the fibres. The diameter used to calculate applied
stress was averaged over the section of fibre where DIC images were
taken. The typical error of diameter is estimated at 4 μm. Young’s
modulus values calculated from the stress-strain curves are plotted
against the fibre drawing tension in Fig.11.
Linear regression applied to the data suggests that drawing stress
may influence the Young’s modulus, with greater stress leading to a
higher modulus. It should be noted however that the gradient of the
line of best fit is 0.017 GPa/MPa while the standard error in the
gradient is almost half this value at 0.008 GPa/MPa, so there is
some uncertainty as to whether there really is a correlation, as
reflected by the correlation coefficient of only 0.37. Further
research is needed to confirm if the two quantities are correlated,
but even if they are, control over the elastic modulus is only
likely to be over a range of perhaps 20% of its nominal value. The
data in Fig.11 also suggest that the annealing process does not
have any significant impact on the Young’s modulus.
Fig.10. Stress-strain curves measured for POF indicated as 1e and
1e'.
Fig.11. Dependence of Young’s modulus upon drawing stress.
Proc. of SPIE Vol. 7714 77140G-7
4. CONCLUSIONS From the presented series of experiments we conclude
that the stress-optic coefficient ΔC in PMMA fibers has negative
sign and with our fibers ranges from -4.5 to -1.5×10-12 Pa-1
depending on the drawing stress. Dependence of ΔC is nonlinear vs.
drawing stress and gradually saturates at greater σdrawing.
Annealing has a significant impact on the dependence of the
differential stress-optic coefficient upon σdrawing. Moreover, our
measurements demonstrate that ΔC is linearly proportional to
initial fiber birefringence with annealing having no impact on the
slope of this dependence. From the DIC measurements, we conclude
that Young’s modulus may only slightly depend on POF drawing
stress. More accurate measurements are necessary to confirm that
result. Moreover, annealing doesn't have impact on Young's modulus
value. Acknowledgements: The work is partly supported by the EU FP7
project PHOSFOS and the Statutory Grant at Wroclaw University of
Technology. M. Szczurowski, G. Satkiewicz-Barabach and W. Urbanczyk
acknowledge support of the FNP Program “MISTRZ”.
REFERENCES
[1] Ohkita, H., Ishibashi, K., Tsurumoto, D., Tagaya A., Koike, Y.,
“Compensation of the photoelastic birefringence of a polymer by
doping with an anisotropic molecule”, Applied Physics A: Materials
Science and Processing 81, 617 – 620 (2005).
[2] Koyama, T., Zhu, Y., Otsuka, T., Takada, T., Murooka, Y., “An
automatic measurement system for 2-dimensional birefringence vector
distribution”, Proc. IEEE, 557 – 560 (1998).
[3] Xu, W., Yao, X. F., Yeh, H. Y., Jin, G. C., “Fracture
investigation of PMMA specimen using coherent gradient sensing
(CGS) technology”, Polymer Testing 24, 900 – 908 (2005).
[4] Waxler, R. M., Horowitz, D., Feldman, A., “Optical and physical
parameters of Plexiglas 55 and Lexan”, Applied Optics 18, 101 – 104
(1979).
[5] Urbaczyk, W., Pietraszkiewicz, K., “Measurements of stress
anisotropy in fiber preform: modification of the dynamic spatial
filtering technique”, Applied Optics 27, 4117 – 4122 (1988).
[6] Primak, W., Post D., "Photoelastic constants of vitreous silica
and its elastic coefficient of refractive index", J. of Appl.
Physics 30, 779 – 788 (1958).
Proc. of SPIE Vol. 7714 77140G-8